Superspace description of the homologous series Ga~2~O~3~(ZnO)~<i>m~</i>
Michiue, Yuichi; Kimizuka, Noboru; Acta Crystallographica Section B 66 (2010) 117–129; doi:10.1107/S0108768109053713

data_2104693
_publ_section_title
;
 Superspace description of the homologous series
 Ga~2~O~3~(ZnO)~<i>m~</i>
;
_journal_coeditor_code           SN5090
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              117
_journal_page_last               129
_journal_paper_doi               10.1107/S0108768109053713
_journal_volume                  66
_journal_year                    2010
_chemical_formula_sum            'Ga0.25 O1.25 Zn0.75'
_chemical_formula_weight         84.5
_chemical_name_systematic        ' ?'
_space_group_ssg_name            Cmmm(00\g)0s0
_symmetry_cell_setting           orthorhombic
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   3.2465(9)
_cell_length_b                   19.640(5)
_cell_length_c                   3.0979(8)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    298
_cell_measurement_theta_max      15.7
_cell_measurement_theta_min      12.6
_cell_modulation_dimension       1
_cell_subsystems_number          2
_cell_volume                     197.53(9)
_computing_publication_material
'Jana2006 (Petricek, Dusek & Palatinus, 2006)'
_computing_structure_refinement
'Jana2006 (Petricek, Dusek & Palatinus, 2006)'
_diffrn_ambient_temperature      298
_diffrn_measured_fraction_theta_full 0.97
_diffrn_measurement_device_type  'Rigaku AFC-7R'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Rotating anode'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.1223
_diffrn_reflns_av_sigmaI/netI    0.1343
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_index_m_1_max 6
_diffrn_reflns_limit_index_m_1_min -6
_diffrn_reflns_limit_k_max       38
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       7
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            7287
_diffrn_reflns_theta_full        24.96
_diffrn_reflns_theta_max         45.02
_diffrn_reflns_theta_min         2.65
_diffrn_standards_decay_%        0.0
_diffrn_standards_interval_count 200
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    24.6
_exptl_absorpt_correction_T_max  0.61
_exptl_absorpt_correction_T_min  0.18
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   'Absorption correction given as psi-scan'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    5.68
_exptl_crystal_description       irregular
_exptl_crystal_F_000             314
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.29
_refine_diff_density_min         -2.27
_refine_ls_extinction_coef       404(14)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_ref   1.03
_refine_ls_number_constraints    4
_refine_ls_number_parameters     115
_refine_ls_number_reflns         3699
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1801
_refine_ls_R_factor_gt           0.0439
_refine_ls_shift/su_max          0.0169
_refine_ls_shift/su_mean         0.0016
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0001I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0683
_refine_ls_wR_factor_ref         0.0988
_reflns_number_gt                1349
_reflns_number_total             3699
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            sn5090.cif
_cod_data_source_block           m=6
_cod_database_code               2104693
_cod_database_fobs_code          2104693